2.3 Influence of water at interfaces
2.3.2 Literature on the influence of humidity on the conductivity of ceria
gives the isosteric heat of adsorption:
The BET-model is based on the following assumptions. (i) The adsorption takes place on fixed sites. (ii) The sites are energetically identical. (iii) No lateral interaction is allowed between the adsorbed molecules. The inclusion of lateral adsorbate-adsorbate interaction leads to the formation of islands.112
With the theoretical background described in this section, in the following two sections the state of knowledge about the influence of water on electrical conductivity of ceria based materials is presented. As the driving forces of chemisorption and physisorption are different, the literature is divided into such works, investigating a temperature regime at elevated temperatures (T?150
◦C) where chemisorption is most likely the relevant process, and those studies with a focus on a lower temperature regime, where physisorption is most likely to occur. Nevertheless, it is emphasized that the transition between the two regime is diffuse.
2.3.2 Literature on the influence of humidity on the conductivity of ceria
Figure 2.10:a) Arrhenius plot of the bulk conductivity determined by Jimenez et al. measured during cooling of the sample. Zirconia rich samples are represented by open symbols. Ceria rich samples are represented by closed symbols. b) Arrhenius plot of heating and cooling cycles. The enhanced conductivity in heating cycles is likely due to residual water in the samples, as they were not stored under dry conditions prior to the first heating cycle.
Measurements are conducted under nominally dry conditions, without drying the carrier gas before streaming into the oven. The residual humidity of 2-3 ppm water content in the gas is sufficient to enhance the conductivity of the samples during the heating cycles. Plots taken from the paper of Jimenez et al. reprinted with permission from John Wiley and Sons.57
Jimenez et al. investigated the influence of temperature,pO2andpH2Orelative pressures on the conductivity of a series of Ce1-xZrxO2(0<x<1) pressed pellets, prepared by solid-state reaction.57The pellets had a relative density of85 %and were contacted with gold electrodes on the larger faces. The temperature range investigated was 120−800°C in heating as well as cooling runs. An YSZ based oxygen pump was used to control and monitor the oxygen partial pressure in the system. A similar setup as it was used for the measurements conducted in the experimental part of the work presented here. Samples were measured under dry and humidified (93% relative humidity) conditions.
Jimenez et al. report a rather complex temperature dependency of the conductivities as a function of temperature, depending on the composition, and whether a heating or cooling experiment was conducted. For cerium-rich pellets two activation energies are found in cooling experiments, as can be seen in figure 2.10. The Arrhenius plots can be divided in two regimes. The first regime is below 850 K approximately, where the slope in the Arrhenius plot is not changing, thus only one activation energy of about 1.5 eV is found, without showing a clear trend with composition. A change in slope is found above 850 K, showing activation energies of3.75−4.5 eV. As Jimenez et al. is not distinct on this aspect the reader has to assume that these measurement cycles were conducted under nominally dry gas conditions with a residual water content of a few ppm. Thus, residual water in the gas atmosphere, which is adsorbed from the laboratory in the open pore volume of about 15%,
most probably influenced the sample conductivity during the heating experiments.Jimenez et al. also conducted measurements in intentionally humidified gas atmosphere. Unfortunately in their paper they did not present the temperature dependence of the conductivity under these conditions. Instead they studied the recovery of the samples conductivity when exposed to humidified gases. They report increasing conductivity in humid gas mixtures, when the sample is held at a constant temperature. Jimenez et al. report that the conductivity of their samples is dominated by electrons. They conclude this from the slopes of the DC conductivity measurements as a function of pO2. An additional indicator for the electronically dominated conductivity is the fact that the imaginary part of the impedance vanishes at low frequencies (< 1 Hz), indicating non blocking electrodes, thus a dominant electronic conductivity.
Jimenez et al. argue that water incorporation can be described by the following reaction, describing the formation of hydroxyl defects.
H2O + V
O + O
In case of Ce1-xZrxO2 the oxygen vacancy concentration [V
O] is not fixed by the dopant concentration, as in gadolinium or samarium doped solid solutions of ceria for example.48,49 Albeit, it is influenced by the surrounding gas atmosphere via extrinsic ceria reduction equilib-rium already introduced in section 2.1.2 equation (11). Hydroxyl defect formation consumes oxygen vacancies (see chemisorption type 1 in figure 2.18) shifting the cerium reduction equi-librium equation (11) to the product site, producing a larger amount of electrons (Ce0
Additionally Jimenez et al. state that water incorporation can also break the associates of oxygen vacancies and electrons (small polarons), increasing the amount of electrons con-tributing to the conductivity. Thus, in humid atmosphere protons and localized electrons are the majority charge carriers. The latter are higher in concentration and mobility, preventing the observation of a dominant proton conductivity at elevated temperatures in the study of Jimenez et al..
The work of Jimenez mainly focuses on a water partial pressure regime, where chemisorption is most probably the transport process, influencing the conductivity of the samples. They investigated nominally undoped ceria pellets. In contrast to that Chueh as well as Haile and coworkers investigated the impact of hydration on the transport properties of micro-crystalline15 mol%samaria doped ceria at higher water partial pressures.49 For this purpose they prepared pressed powder pellets of the material with a density of ≈95 % by a classic solid state reaction route. Impedance spectroscopy measurements in the temperature range of 650−250°C under H2O saturated and D2O saturated conditions were conducted under oxidizing and reducing conditions. By separating bulk from grain boundary contribution,
Chueh et al. were able to observe that under oxidizing conditions humidification caused a substantial increase in the grain boundary resistivity while the bulk impedance remained unchanged. The results under H2O and D2O hydration were identical in the temperature regime between 450−250°C. The transport process involved showed a higher activation energy under humidified conditions. With decreasing temperature the impact of hydration became larger, as well as with increasing humidity.
In contrast to the conductivity enhancement often reported for oxides under humidified con-ditions, like Jimenez reported as well (discussed above), Chueh et al. report a decrease in conductivity for Sm doped ceria and explain this effect with the motion of hydroxylic or protonic species being the reason for the enhancement of the surface and grain boundaries conductivity. They argue with an combined brick layer and space-charge model, where the space-charge layer thickness decreases with the samaria concentration. From the mean grain size and the capacity ratio between grain interior and grain boundary, the space charge width was determined to be 0.8−1.2 nm under dry conditions at 250
◦C. This is approximately two times the lattice constant of doped ceria. Chueh et al. assume the grain boundary core to be ion-reversible, as the grain boundary resistance increase upon humidification is a property not expected for transport limited by the core itself. This assumption was also made by Avila-Paredes et al., when they studied gadolinium doped ceria.52
With this assumption Chueh and coworkers calculated the increase of the space-charge po-tential to be 5−6 mV in the investigated temperature range. This increase in Φ leads to a change in [V
O] upon humidification. Depending on the boundary conditions chosen, the space-charge potential change varies around 0.5 %, leading to a4 %difference in the oxygen vacancy concentration, that decreases by about 24−28 % upon hydration. The magnitude of the space-charge potential increase depends on whether there is a proton uptake from the bulk or not. In case of bulk proton uptake one would assume a depletion of protons in the SCL, while the oxygen vacancy depletion would still be more significant.
A positive ∆Φ implies that the positive charge transported by cations in the grain boundary core is larger than that transported by anions. This effect can be described when anion sites in the core, that should be occupied by oxide ions, are occupied by hydroxyl groups instead, which are less negatively charged than oxide ions. The situation in microcrystalline doped ceria is different than that described in literature for nanocrystalline materials where proton transport via the grain boundary core in direction parallel to the current is reported to become dominant at low temperatures.45,48,58,114,115
So far, only studies on pressed powders were discussed. In order to have a better control of the porosity, researchers started to investigate thin films as model systems. A remarkable work on thin films is the study by Oh and coworkers from the research group of S. Haile.38
They prepared two nominally undoped ceria thin films by MOCVD methods and investigated the resistivity of their nanocrystalline columnar thin films, while varying the water partial pressure and the temperature systematically. This work is one of the rare works that used nanocrystalline columnar thin films with well known morphology, rather than using pressed pellets, whose density varies due to particle size, morphology and preparation technique. The 5.6µmthick thin films prepared showed a30 %porosity (see figure 2.11a)). The conductivity measurements were done by EIS in a macroscopic two point electrode setup. The conduc-tivity was thus measured through the thin film and the substrate, parallel to the columnar crystallites the film consisted of. The humidity was controlled by saturating high purity oxygen with water held at a specific temperature. The measurements were carried out by first heating the samples to 500
C at first. After the impedance spectra were stabilized, the temperature was lowered with a ramp rate ≤2°C/min between dwells of ≥30 min.
Under these measurement conditions Oh and coworkers found that increasing the humidity introduces a medium frequency arc for a small p(H2O) window only, that could not be fitted by means of standard equivalent circuit routines. Thus, they evaluated the impedance of the high frequency semicircle that they interpreted as a mixed response of the grains and the bulk. For polycrystalline, macroscopic samples, one often finds two distinct semicircles, one at high frequencies representing the bulk response, and one at slightly lower frequencies representing the grain boundaries. This does not hold necessarily for nanocrystalline thin films, as the space charge zones could overlap like already mentioned in section 2.2.95,96,102 As the two contributions could not be separated, Oh et al. analyzed the resistance asso-ciated with the thin film response (bulk and grain boundaries). They found a increase of the conductivity with increasing water partial pressure in the temperature regime between 400−200
◦C. This is the opposite of what Chueh et al. reported.49 Oh et al. interpreted the resistive element to correspond to proton migration along the surface of the parallel grain boundaries and/or open surfaces. Plotting the resistivity against the water partial pressure in the atmosphere around the sample (see figure 2.11 b) ) shows a slope close to −3
4 in the double-logarithmic form. Oh et al. conclude, that according to equation (36), describing the proton incorporation reaction, one would expect a power law factor of −1
2. This factor was reported for proton conducting Gd-doped ceria at 200
C by Ruiz-Trejo and coworkers before.48 Their studies were - like most of the work in literature - conducted on macroscopic pellets, with a less specific morphology, but a density of about 90 %. However, Oh et al.
found a deviation from this power law and argue that the main reason is the low oxygen vacancy concentration in nominally pure ceria, leading to site saturation effects, which are not further discussed in their paper. Furthermore, they state that the characteristics found in the resistivity data should reflect the adsorption isotherm of nanocolumnar ceria. A
state-Figure 2.11: a) SEM cross section image of the nanocrystalline columnar thin film prepared by Oh and coworkers.38The film thickness is≈5.6µm. b) Resistivity of a nominally undoped nanocrystalline ceria thin film at different temperatures as a function of the water partial pressure. The slopes of the doubly logarithmic graphs are close to −3
4. Both images are taken from the paper discussed in this paragraph.38 Reproduced from Ref.38with permission from the PCCP Owner Societies.
ment that is addressed later in this thesis, as simulations of conductance data at various water partial pressures based on adsorption isotherms and percolation theory for the temper-ature regime T . 150
C are part of the data interpretation. Oh et al. conclude that their results show proton transport occurring along the exposed grain surfaces and parallel grain boundaries, as no impedance due to grain boundaries normal to the direction of transport is observed.38
A further study on thin films was conducted by Gregori et al..46 They studied epitaxial as well as dense and porous nanocrystalline thin films of ceria and 10 mol-% Gd-doped CeO2, in order to evaluate the influence of residual pore volume on the conductivity enhancement due to proton conductivity. This is one of the rare works in this field, using thin films with controlled porosity as a model system. The films exhibit a thickness in the range of 200−400 nm. Their porosity was controlled by the preparation technique. Epitaxial and nanocrystalline dense films were prepared by PLD, whereas non dense nanocrystalline films were prepared by spin coating. The crystallite size of the spin coated film, was in the same range of the lateral crystallite size of the columnar grown PLD films. The films were con-tacted with parallel platinum electrodes and measured under dry (using a cold trap) and wet (p(H2O) = 20 mbar) conditions. This study is one of the rare studies, that presents data on the conductivity of all thin film types over a large temperature range from 500−30°C.
For the higher temperature region above 100
C Gregori et al. do not observe a significant difference between the nanocrystalline and epitaxial GDC thin films. Though quite
remark-able there is a slight decrease in conductivity of the pure CeO2 samples (nanocrystalline and epitaxial) under dry conditions compared to wet conditions, which is not discussed further within the paper. In the low temperature region(T<50°C under wet conditions the conduc-tivities increase drastically for the epitaxial and the nanocrystalline dense samples. Gregori et al. attribute this conductivity enhancement to condensation of water on the top surface.
For the porous samples the behavior in dry atmosphere is very similar to that of the other films under investigation. However, there is a significant conductivity enhancement, already at temperatures T<300°C, in wet atmosphere. The conductivity difference between wet and dry conditions becomes more pronounced at lower temperatures as shown in figure 2.12.
This findings confirm previous studies on the proton conductivity in nanocrystalline nomi-nally pure and 6 mol% Gd doped ceria (GDC) by Shirpour and coworkers.58 Shirpour and Gregori both conducted their research in the group of Joachim Maier in Stuttgart. Gregori et al. discuss in detail whether the proton conduction along the open pore walls is due to proton injection of protons into the material in the space charge zone below the surface, or whether conduction occurs predominantly within the water layer adsorbed on the surface of the pores. They conclude that proton conduction within the water layer adsorbed on the walls of the open porosity is absolutely plausible. This conclusion was made from an estima-tion of reasonable proton mobilities based on the brick layer model for percolating porosity using the following equation.18
d φPσ∞,L (37)
Hereais the thickness of the adsorbed water layer,dis the average pore size,σ∞,L is the bulk proton conductivity and φP is the open porosity volume fraction ranging from 0.05−0.3.
Thus, regarding to this work, the residual open porosity of the thin film sample is the key factor for the protonic conductivity, rather than the large grain boundaries density, as a dense nanocrystalline thin film does not show a conductivity enhancement below300
◦C. It remains unresolved whether the conduction occurs in the water layer on the surface or within the solid oxide space charge zone right at the interface between water and ceria.
In contrast to Chueh and coworkers who investigated microcrystalline material, Avila-Paredes et al. investigated nanocrystalline ceramics of GDC with an average grain size of 15 nm.52 Their main focus was the temperature regime between 400−30
◦C, in which they investi-gated the conductivity as a function of the dopant concentration. This temperature range seems reasonable in order to detect all effects probably caused by adsorbed water. They prepared nanocrystalline ceria pellets doped with 0.5, 10 and 20 mol% gadolinium and mea-sured the bulk resistance by EIS under dry and wet conditions. Their results are shown in figure 2.13.
Figure 2.12:Main result (and graph) taken from the study by Gregory et al. reprinted with permission from John Wiley and Sons.46The conductivity of a porous CeO2film under wet conditions b) starts increasing at T<300°C already, while a dense film a) only shows conductivity enhancement atT<50°C.
Figure 2.13: Main results of the work by Avila-Paredes and coworkers reprinted with permission from the Royal Society of Chemistry.52 The total conductivity of GDC is dominated by the dopant concentration above 200
◦C. Below 200
C proton conductivity becomes dominant, without being a function of dopant concentration or grain size.
They found that the conductivity above 200
C is clearly dependent on the Gd dopant concentration, as the total conductivity of the sample at these high temperatures is mostly dominated by the oxygen vacancy concentration and not by adsorbed water. At temperatures below 200
C the total conductivity becomes dominated by the proton partial conductivity.
The conductivity for low temperatures under wet conditions is the same for any composition.
This stresses the fact that both the proton concentration and their mobility are not influenced by the dopant concentration. Thus, the bulk defect chemistry described by equation (36) is irrelevant for grain boundaries or interfaces, as there is no connection detectable between dopant concentration in the bulk phase and the proton concentration in the grain boundaries.
This statement somewhat contradicts the idea of a space-charge layer in which the charge carrier concentrations are determined mainly by the space charge.
Avila-Paredes carried out the same experiment with nanocrystalline 8 mol-% yttria stabilized zirconia with crystallite sizes between 13−100 nm and found a non-linear dependence of the conductivity at temperatures below 150
C on the mean grain size d of their powder samples:53
σ ∝ d−nwithn ≈3 (38)
Avila-Paredes state that if the brick-layer is a good approximation for microcrystalline struc-tures the grain boundary conductivity should increase by one too two orders of magnitude if the grain size decreases from 100−10 nm. An effect that cannot be explained by the grain boundary density only. Avila-Paredes and coworkers therefore suggest changes in the defect distribution, leading to a charged grain boundary core, with an corresponding SCL to be responsible for the non linear behavior.
Interestingly these works are cited by Chueh et al.49 in order to back up their theory of an ion-reversible grain boundary core as the reason for the grain boundary resistance increase upon humidification at elevated temperatures. A statement that is vague as Avila-Paredes and coworkers argue for a different temperature range.
From the context of operating SOFC’s at temperatures below the usual 800−1000
C in order to overcome technical obstacles and degradation problems Sangtae Kim and Manfred Martin together with their coworkers searched for alternatives to be operated at lower tem-peratures.45 They build a water concentration cell using yttrium stabilized zirconia (YSZ) as a proton conducting electrolyte operating at room temperature. For that purpose they pressed nanostructured YSZ and SDC (20 mol-% samarium) dense pellets and measured the electromotive force (emf) when one side of the cell was exposed to dry air, while the other side was exposed to moist air or even dipped into liquid water. They measured emf values of up to 200 mVacross the electrolyte and steady state currents of 30 nA. Reducing the grain
Figure 2.14:Short circuit currents measured in water concentration cells with nano- and microstructured 20 mol % SDC and 8 mol % YSZ at room temperature by Kim and coworkers. A Nano-SDC concentration cell delivers a remarkable current of 30 nA. Figure taken from the publication of Kim et al. reprinted with permission from John Wiley and Sons.45
size in the pellets by sintering the starting material, the emf measured in a concentration cell was the same, than for nanocrystalline material, but the currents measured on a short-circuited cell were smaller than 10 pA. Whether this decrease was only due to a change in the geometric scaling factor or due to a change in the nature of the grain boundary region was not elucidated by Kim et al.. For further proof that SDC and YSZ actually conducted protons, secondary ion mass spectrometry measurements were conducted on samples ex-posed toD2Osaturated air. A summary of these findings is shown in figure 2.14 taken from the respective paper.45 The power output of the concentration cells is qualitatively similar to those of classical SOFC’s but unfortunately the power densities in those cells are low.
Takamura and Takahashi describe the water adsorption behavior and electrical conductivity of 6 mol-% SDC nanoparticles.115 They used volumetric water vapor adsorption at room temperature as well as thermogravimetry analysis (TGA) to study the adsorption behavior of nanoparticles powder samples with crystallite sizes below 50 nm. They compared a sam-ple prepared by homogeneous precipitation using hexamethylenetetramine (HMTA) with a sample prepared by UV laser irradiation of a cerium and samarium nitride solution. For the HMTA sample they found a large amount of water adsorption reaching up to3 mass−% at very low water pressures of only368 Pathat most probably are often referred to as dry condi-tions in other works. Under the same condicondi-tions the UV sample only showed0.12 mass−% water adsorption. From BET measurements Takamura and Takahashi conclude that this is mostly due to secondary particle size differences of the powders. A noteworthy observation in this study is, that the electrical conductivity of both samples, HMTA and UV, which show